Help Line tech
877.727.7443 Ink Chalk and Scuff tips
although the printed ink film is dry, residual ink pigments transfer to where
they are unwanted, usually onto unprinted areas of the paper; or ink and pa-
per visibly mark through the mechanical action of rub or abrasion.
Ink scuff is often described in other terms such as marking, chalking, ink
rub, and setoff. although the latter term more typically defines the non-me-
chanical action of wet ink offset, ink scuff refers to the transfer of dry ink
pigment through the abrasive mechanical action of contact and rub. Ink
chalking and surface abrasivity are the primary mechanisms contributing to
ink scuff. If ink holdout is especially low and the ink penetrates too deeply
into the paper surface, ink vehicles may drain off the resins, dryers, and
waxes that would normally “bloom” to the surface to solidify the pigments.
This condition, which also can retard ink dry, is known as ink pigment filtra-
tion and usually results in ink chalk and scuff.
The three primary components of ink scuffing are:
1. Ink film resiliency – after properly transferring to the plate, blanket, and
paper, the conventional sheetfed ink film must effectively set, which is de-
fined as the physical loss of ink solvent as it absorbs into the substrate. The
second phase is the chemical process of actual ink dry through oxidative po-
lymerization. In contrast, web heatset inks dry by evaporation, utilizing dryer
heat to evaporate the unabsorbed ink solvents and a chill-roll system to gel
and set the melted ink resins. Sheetfed inks, with higher levels of oxidizable
resin, are considered much more durable and scuff resistant than web heat-
set inks. In either case, effective ink set must allow the ink vehicle to “bloom”
the resins, dryers, and waxes to the surface to properly bond with the pig-
ments during the drying process.
2. Paper smoothness and hardness – Matte, silk, satin, and dull coated papers
typically have a rougher surface which creates an abrasive rub making these
papers more susceptible to marking and scuff. In addition, rougher or soft-
surfaced papers, in conjunction with certain quick-set ink formulations, can
absorb ink solvents much quicker and deeper than smoother tight-surfaced
substrates creating the potential for ink pigment filtration. These compound-
ing characteristics can make ink scuff and marking a definite concern.
3. Mechanical action – areas of the printed piece that experience the most
pressure and contact may rub too roughly through post-print production pro-
cesses. Ink scuff is usually worse near folds, bulky spines, or shingled pages.
Ink scuff and marking can occur through equipment contact with wheels,
nips, and belts through the feeding, delivery and finishing processes.
Ink Chalk and Scuff (continued)
• Ink formulation and/or ink set rate not compatible with absorbency rate of
paper. Ink sets too deep resulting in ink pigment filtration.
• Unprotected coarse-ground ink pigments such as reflex blue and metallic
• Lack of wax or slip agents in the ink formulation.
• Ink dries too slowly. Conditions that may compromise ink set and dry
Incompatible set rate of ink and paper.
High relative humidity in the pressroom (over 60%).
Improperly conditioned paper (i.e., cold paper in a heated pressroom).
Paper absorbing excessive moisture transferred from the plates.
Over-emulsified ink from excess water or high-acid fountain solution.
High acidity of fountain solution compromising ink drier.
High conductivity of fountain solution compromising effective ink set.
Too much or too little drier in the ink.
• Substrate surface is rough and abrasive.
• excessive use of anti-offset spray powder causing abrasive contact points
for scuffing in transit.
• Lack of protective overcoat.
• Dull varnish over unprinted paper. Most dull varnishes are formulated with
coarse-ground dulling agents, which are both abrasive and susceptible to
surface filtration during the setting process. In addition, these dulling agents
are hydrophilic and tend to take on water which can retard the ink drying
process. These characteristics, in conjunction with the abrasive nature of
soft-surfaced papers, can be very problematic, especially when dull varnish
is used without the benefit of cross-linking with a wet ink film.
• High contact paper-to-ink or paper-to-equipment rub pressure during pro-
• Loose packaging inducing high-contact rub and movement during
Options and Solutions
• Ink set rate should be compatible with absorbency of the substrate sur-
face. a tighter-surfaced, high-holdout substrate may require a quick-set ink,
whereas, a more absorbent soft-surfaced substrate may demand a less in-
teractive and slower ink set to increase holdout and improve “hard-dry”
• Coarse-ground ink pigments, such as metallics, should be protected with
either a varnish, aqueous, or UV over-coat.
• When over-coat and post-press applications permit, the inclusion of Teflon
wax in the ink formulation will improve ink resiliency and surface slip.
Ink Chalk and Scuff (continued)
• For timely and thorough ink dry consider the following best-practices:
Select the ink formulation best suited for the job and substrate. Do not
alter inks without consulting with ink supplier.
Ideal pressroom environment is 45% (+/-5%) RH @ 72° F. for North amer-
ica and 52% (+/-5%) Rh @ 21° C. for europe (See Sappi tech tip on Paper
Conditioning & Characteristics).
allow paper to fully acclimate to recommended pressroom environment
before unwrapping. Paper acclimation is relative to volume of paper and
environmental extremes, but the industry-accepted best-practice is 24-
Optimize ink/water balance and minimize water to the plate whenever
Fountain solution should be buffered to a pH no lower than 4.0 (european
printing systems tend to run more alkaline recommending a pH value no
lower than 4.8).
Consult with fountain solution supplier for appropriate conductivity of
“Wind” printed loads in small lifts after ink has sufficiently set.
• Cover grades and more absorbent matte, dull, and silk finishes may de-
mand special consideration to improve ink film resiliency and minimize scuff
Inks typically known as “hard-dry” or “cover set” formulations may con-
tain additional oxidizable resins and/or Teflon waxes.
although not as hard and resilient as sheetfed inks, web heatset inks,
which dry by evaporation, may be formulated with small amounts of
drying oils which will allow for additional post-press hardening through
oxidative reaction. Consult with ink supplier.
Most importantly is the consideration of a protective UV, aqueous, or var-
nish overcoat. Gloss varnishes offer more surface resiliency and better
scuff resistance than dull varnishes. a satin varnish with at least 60% gloss
in the formulation is usually considered the best compromise for a dull ef-
fect. The best options for overcoat surface protection are as follows:
Since web heatset ink lacks the resiliency of sheetfed ink, it may be nec-
essary in some heavy coverage web heatset print applications to overall
varnish both image and non-image with a gloss or satin varnish to in-
crease ink-to-paper slip.
• The use of spray powder can be beneficial in maintaining sheet separation,
but keep micron size and dispersion volume as small and light as possible
to prevent it from becoming an abrasive agent.
Ink Chalk and Scuff (continued)
• avoid running straight dull varnishes over unprinted paper. an industry-ac-
cepted compromise to reduce high-glare gloss is the use of satin varnish
with at least a 60% gloss varnish in the formulation. If the project demands
a maximum dull image effect, consider a strike-through dull varnish ap-
plication, which allows for a protective, in-line gloss aqueous overcoat.
Consult with ink supplier regarding the need for a special strike-through dull
• Scrutinize printed material during all post-print production processes to de-
termine areas of high contact and scuff, and backtrack through the process
to decrease or move any undue pressure or contact. Keep rubbing to a
• Consider slip-sheeting finished pieces to minimize potential ink scuff around
high contact areas such as spines, folds, and embossed surfaces.
• Shrink-wrap or package finished pieces as tightly as possible to avoid po-
tential movement during transit.
Production tips for printing on matte, dull, satin and silk paper
Soft, warm, and inviting, matte, dull, satin, and silk finished papers have
their own set of production needs. The very surface and finish qualities that
make them attractive, including their good opacity and bulk, their readable,
writeable, non-glare surface, also make marking/scuff a concern. Formulat-
ing hard dry inks can help reduce scuffing concerns.
additionally, applying a protective overcoat will prevent inks from rub-
bing off onto facing pages. Finally, consider protecting your covers with
slip-sheets or envelopes, especially when covers are embossed.